Lee, S. Y.104 Pertanika J. Sci. & Technol. Vol. 20 (1) 2012(1-5wt%) of nanometric-sized clay particles. The objectives of this study were to investigate theinfluence of screw configurations and barrel temperatures on the RTD and to analyze the influence ofextrusion variables on the MRT and variance of RTD affecting the properties of the nanocompositefoams. In this article, emphasis is given on the RTD results and the influence on MRT and variance,whilst the properties are not discussed.MATERIALS AND METHODSMaterialsSemicrystalline poly(lactic) acid (PLA) resin of MWn 85,000 was produced by Cargill, Inc.(Minneapolis, MN, USA). Commercially available tapioca starch was purchased from StarchTech, Inc. (Golden Valley, MN, USA). Organoclay, under the trade name of Cloisite 10A, waspurchased from Southern Clay Co. (Gonzales, TX, USA) and used as nanofiller. The organoclaywas organically-modified montmorillonite (MMT). Tapioca starch was agglomerated into sphericalgranules of 2-4mm diameter to facilitate feeding into the extruder. The moisture content of thetapioca starch was adjusted to 20%, dry basis, with distilled water prior to extrusion. Tapioca starchand PLA(90:10 weight ratio) were blended with 3% Cloisite 10Ain a Hobart mixer (Model C-100,Horbart Corp., Troy, OH, USA) and stored in plastic bottles prior to extrusion.ExtrusionAtwin-screw extruder (model DR-2027-K13, C. W. Brabender, Inc., S. Hackensack, NJ, USA), withtwo types of corotating screws (namely, compression and mixing screws, model CTSE-V, C. W.Brabender, Inc., S. Hackensack, NJ, USA) was used to conduct the extrusions. The conical screwshad diameters decreasing from 43mm to 28mm along their length of 365mm from the feed endto the exit end. The compression screws were universally single flighted corotating intermeshingscrews with interrupted flight mixing zones. The mixing screws had a mixing section, in whichsmall portions of the screw flights were cut away. The mixing section enhanced the mixing actionand also increased the residence time of the sample in the barrel. A 90-rev/min screw speed wasused for all the extrusions. The temperature at the feeding section was maintained at 50°C, whilethe second barrel section at 120°C and the third barrel section and die section were maintained at150°C. Die nozzle of 3mm diameter was used to produce extrudates which were cut by a rotatingcutter. The extruder was controlled by a Plasti-Corder (Type FE 2000, C. W. Brabender, Inc. S.Hackensack, NJ, USA). Data including barrel temperature profiles, pressure profiles and torquereading were recorded by a computer for subsequent analyses. Extrusion conditions selected werebased on the preliminary studies and previous experiments.Determination of RTDThe RTD study was performed using a dye technique (Lin & Armstrong, 1990). The tracer usedfor determining the RTD was prepared by mixing 0.05g of red dye sodium erythrosine (SigmaChemical Co., St. Louise, MO, USA) with 5g of tapioca starch and the amount of water neededto bring the moisture content of the tracer to that of the feed material (20%) (Lee & McCarthy,1996). The tracer was added as a pulse input through the inlet port of the extruder when steady stateconditions were achieved. Foam samples were collected every 5s for 3 min after adding the tracer.
Residence Time Distribution of Tapioca Starch-Poly(lactic acid)-Cloisite 10ANanocomposite Foams in an Extruder105Pertanika J. Sci. & Technol. Vol. 20 (1) 2012ColorimeterThe 5 s samples were ground in a mill to pass through a 50 US standard sieve. The values of L*a* b* were measured three times for each ground sample using a Chroma meter (Model CR-300,Minolta, Japan). The red colour intensity, c was calculated as:c a b2 2= +) )^ ^h h where a* represents the value of redness and b* is the value of blueness. However, the value of b*did not contribute to the red colour intensity (Seker, 2005), so c was simplified as:c = a* Thus, the value of the redness, a*, was used as a measure of red colour intensity of the tracerconcentration in the extrudate (Bi et al., 2007).RTD FunctionsIn general, RTD can be described with two functions, namely, E(t) and F(t) diagrams, which areclosely related (Levenspiel, 1972). The response of the extruder to a pulse at the inlet is given by theE(t) diagram, which represents the age distribution of the material in the extruder. Since it is difficultto ensure that the same amount of tracer is used in all the experiments, it is common to normalizethe tracer concentrations at each point in time by dividing them by the total amount of tracer passingthrough the system. Thus, the E(t) diagram can be obtained by dividing the concentration, at anytime interval, by the total amount of tracer injected, as given in the following equation:E ti c dtcc tciiiiii00T.==3 3==^ h/#where c is the tracer concentration at time t.The F(t) diagram is related to the E(t) diagram and it represents the cumulative distributionfunction in the exit stream at any time.F tc tE t dtc tiiiiii tii t000 TT,= 3..====^ ^h h//# The mean residence time (MRT) or (t ) which represents the mean time that a particle spentin the extruder can be described as:t t E t dtc tt c tiii tiii ii000TT,= 33...=^ h//# 
Lee, S. Y.106 Pertanika J. Sci. & Technol. Vol. 20 (1) 2012While the variance (σ2) can be described as:c tt t c tiiiii2002TT,v-33..^ h//Experimental Design and Statistical AnalysesA 2 x 2 factorial design (with three replications) was used to analyze the effects of screwconfigurations (compression and mixing screws) and barrel temperatures (150 and 160ºC) on theRTD. The results for the measurements were analyzed using the general linear models (GLM) inthe SAS analysis program (SAS Institute Inc., Cary, NC, USA). Duncan’s multiple range tests wereconducted to check for significant (p<0.05) differences between the treatment groups.RESULTS AND DISCUSSIONRTD is a key parameter for characterizing the performance of an extruder reactor. A twin screwextruder often works under starved conditions. Thus, screw configurations and temperature are twoindependent operating parameters. Their respective influences on the RTD measured by the abovedescribed method are shown in Fig. 1. As expected, for a given screw configuration, an increasein temperature shifted the RTD function to the short time domain. For a given temperature, themixing screw displayed a similar effect. All the RTD curves were of good quality, regardless ofthe screw configurations and/or temperature. This implies that the extruder is able to work under arelatively large processing window. Meanwhile, the reproducibility of the experiments carried outin the present study was found to be very good, as shown in Fig. 2. The figure shows that the RTDfor two experimental runs at the same operating conditions were almost identical.Fig. 1: Residence time distribution of (a) mixing screws at 150ºC, (b) mixing screws at160ºC, (c) compression screws at 150ºC, and (d) compression screws at 160ºC.
Residence Time Distribution of Tapioca Starch-Poly(lactic acid)-Cloisite 10ANanocomposite Foams in an Extruder107Pertanika J. Sci. & Technol. Vol. 20 (1) 2012The influences of screw configurations and temperature on MRT are shown in Table 1. TheMRTs were significantly different (p < 0.05) for mixing and compression screws at 150ºC and160ºC, respectively. As expected, the mixing screws had longer MRT than the compression screws.In addition, lower temperature resulted in longer MRT for both screws, as expected. On the otherhand, higher temperature produced more heat energy which decreased the viscosity of the mass,resulting in a more flowable material. Similar results were also reported by Altomare et al. (1986).Data from mixing screws at 150ºC had significantly higher variance. However, the MRTs werenot significantly different for the compression screws at 150ºC and 160ºC. Similarly, the varianceswere not significantly different for both sets of screws at 150ºC and 160ºC.TABLE 1Mean residence time (MRT) and variance for mixing and compression screws attwo temperaturesTemperature [ºC] MRT [s] Variance [s2]Mixing 150 110.7a 1008aMixing 160 98.74b 750.2bCompression 150 91.74c 734.5bCompression 160 83.43d 658.5ba-dmeans with same letter within a column indicate no significant (P>0.05) difference byDuncan multiple range test.CONCLUSIONSIn this study, the RTD results produced curves with good distribution, which is related to the MRTof the process. The influences of screw configuration and temperature on RTD were predicted wellusing the process. Mixing screws had longer MRT compared to the compression screws. LowerFig. 2: Residence time distribution of mixing screws obtained at the same operatingconditions (a) 150ºC and (b) 160ºC for two experimental runs.
Lee, S. Y.108 Pertanika J. Sci. & Technol. Vol. 20 (1) 2012temperatures resulted in longer MRT for both the screws. Mixing screws at 150ºC had significantlyhigher variance. Nevertheless, the variances were not significantly different for both sets of thescrews at 150ºC and 160ºC.ACKNOWLEDGEMENTSThis research was funded by University of Nebraska Agricultural Research Division, supportedin part by the funds provided through the Hatch Act, USDA. Our sincere thanks are due to Prof.Dr. Milford Hanna of University of Nebraska, Lincoln and Malaysian Agricultural Research andDevelopment Institute (MARDI) for supporting this work.REFERENCESAltomare, R. E., & Ghossi, P. (1986). An analysis of residence time distribution patterns in a twin screwextruder. Biotechnology Progress 2(3), 157-163.Bi, C., Jiang, B., & Li,A. (2007). Digital image processing method for measuring the residence time distributionin a plasticating extruder. Polymer Engineering Science 47, 1108-1111.Chen, L.G. Hu, H., & Lindt, J. T. (1995). Residence time distribution in non-intermeshing counter-rotatingtwin-screw extruders. Polymer Engineering Science, 35, 598-603.Fichtali, J., & van de Voort, F. R. (1989). Fundamental and PracticalAspects of Twin Screw Extrusion. CerealFoods Worlds 34, 921-929.Gao, J., Walsh, G., Bigio, C. D., Briber, R. M., & Wetzel, M. D. (1999) Residence-time distribution model fortwin-screw extruders. AICHE Journal 45(12), 2541-2549.Gogoi, B. K., & Yam, L. K. (1994). Relationship between residence time and process variables in a corotatingtwin-screw extruder. Journal of Food Engineering, 21, 177-196.Lee, S. Y., & McCarthy, K. L. (1996). Effect of screw configuration and speed on RTD and expansion of riceextrudate. Journal of Food Process Engineering, 19, 153-170.Levenspiel, O. (1972). Chemical Reaction Engineering (2ndEd.). N.Y.: Wiley.Lin, J. K., & Armstrong, D. J. (1990) Process variables affecting residence time distributions of cereals in anintermeshing, rounter rotating twin screw extruder. Transaction of ASAE, 33, 1971-1978.Seker, M. (2005) Residence time distributions of starch of high moisture content in a single screw extruder.Journal of Food Engineering, 67, 317-324.Todd, D. B. (1975) Residence Time Distribution in Twin-Screw Extruders. International Polymer Processing,6, 143-147.Wolf, D., Holin, N., & White, D. H. (1986) Residence time distribution in a commercial twin-Screw Extruder.Polymer Engineering Science, 26, 640-646.